Three-Dimensional Metal-Free Molecular Perovskite with a Thermally Induced Switchable Dielectric Response.
Chu, Lu-Lu; Zhang, Tie; Zhang, Wan-Ying; Shi, Ping-Ping; Gao, Ji-Xing; Ye, Qiong; Fu, Da-Wei; The journal of physical chemistry letters  (2020) 1668–1674; doi:10.1021/acs.jpclett.9b03556

data_8000419
_publ_section_title
;
 Three-Dimensional Metal-Free Molecular Perovskite with a Thermally
 Induced Switchable Dielectric Response.
;
_journal_name_full               'The journal of physical chemistry letters'
_journal_page_first              1668
_journal_page_last               1674
_journal_paper_doi               10.1021/acs.jpclett.9b03556
_journal_year                    2020
_chemical_formula_moiety         'B3 F12 Rb, C6 H14 N2'
_chemical_formula_sum            'C6 H14 B3 F12 N2 Rb'
_chemical_formula_weight         460.09
_space_group_crystal_system      cubic
_space_group_IT_number           205
_space_group_name_Hall           '-P 2ac 2ab 3'
_space_group_name_H-M_alt        'P a -3'
_atom_sites_solution_hydrogens   mixed
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   14.2492(2)
_cell_length_b                   14.2492(2)
_cell_length_c                   14.2492(2)
_cell_measurement_reflns_used    986
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.8560
_cell_measurement_theta_min      2.8340
_cell_volume                     2893.15(7)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'XtaLAB Mini II'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0738
_diffrn_reflns_av_unetI/netI     0.0621
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            4295
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        24.946
_diffrn_reflns_theta_max         24.946
_diffrn_reflns_theta_min         2.476
_exptl_absorpt_coefficient_mu    3.555
_exptl_crystal_density_diffrn    2.113
_exptl_crystal_description       block
_exptl_crystal_F_000             1792
_refine_diff_density_max         0.377
_refine_diff_density_min         -0.858
_refine_diff_density_rms         0.095
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.082
_refine_ls_hydrogen_treatment    refU
_refine_ls_matrix_type           full
_refine_ls_number_parameters     81
_refine_ls_number_reflns         854
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.082
_refine_ls_R_factor_all          0.0832
_refine_ls_R_factor_gt           0.0528
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0590P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1153
_refine_ls_wR_factor_ref         0.1275
_reflns_Friedel_coverage         0.000
_reflns_number_gt                572
_reflns_number_total             854
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            jz9b03556_si_004.cif
_cod_data_source_block           1
_cod_depositor_comments
'Adding full bibliography for 8000416--8000419.cif.'
_cod_original_cell_volume        2893.15(12)
_cod_database_code               8000419
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              3649
_shelx_hkl_checksum              88463